compressibility of natural and synthetic high polymers at high
Post on 04-Jan-2017
Embed Size (px)
Journal of Research of the Notional Bureau of Standards Vol. 46, No.3, March 1951 Research Paper 2192
Compressibility of Natural and Synthetic High Polymers at High Pressures
Charles E. Weir
Co mpressio n data ( - t. V IVo) are repor ted between 1,000 and 10,000 atmospheres for the foll owing materi a ls : dry cellulose, polyvinylidene chloride (Saran), polyethylene, poly-rnonochlorotrifluoroethylene (Kel-F) , polytetrafluoroethylene (T efion), a polyester (Seleetron 5003), and raw r ubbers, H ycar OR25, H ycar ORIS, Neoprene, a nd Thiokol ST . All com-pression curves are smooth excep t that for polytetrafiuoroethylene, which shows a transition at 5,500 a t mospheres, resulting in a change in volume (t. V IVo) of approximately 2 percent. Coefficients of t he cubic eq uat ions, - t. V IVo= a(P - 2000) + b (P - 2000)2 +C (P - 2000)3 fi tted to t he data are as follows: Cellulose: a = 9.26 X 10- 6 , b=-3.25 X 10- 1O, c= 2.93 X 10- 's; polyvinyJidene chloride (Saran) : a = 2.17 X 10-s, b=- 1.90 X IO- 9, c= 8. 73 X lO- l4 ; poly-ethylene: a = 1.89 X IO- s, b=- 1.45 X IO- 9, c= 6.lO X lO- 14 ; polymonochlorotrifjuoro-ethylene (Kel-F): a = 9.89 X lO- 6, b=-4.74 X lO- 1O, c= 8.29 X lO- ' 5 ; polyester (Selectroll 5003) : a = 1.76 X lO- s, b=- 1.23 X 10- 9, c= 4.82 X lO- 14 ; H ycar OR25: a = 2.26 X IO-5, b= - 2.03 X lO- 9, c= 9. 09 X IO- I4 ; H ycar OR15: a = 2.17 X 10- 5, b=- 2.03 X lO- 9, c= 9.42 X IO- I4; Neoprene: a = 2.04 X IO- s, b=- 1.75 X 10- 9, c= 7.66 X 10- 14 ; Thiokol ST : a = 1.92 X 10- 5, b= - 1.41 X 10- 9, c= 6.07 X 10- 14 Co mprcssibilities calculated from these eq uations s how fictitious minima cir ca 10,000 atmosphere, although t he eq uations represen t the data satis-factorily to 10,000 atmospheres. The data given compare favorably with those obtained 0 11 similar materials by previou workers.
In a previous paper  1 the design, constru ction , and use of apparatus for measuremen t of volume change of solids (or liquids) at high pressure wa described . The apparatus was applied to a deter-mination of the compression of leather and collagen in the forementioned report. This equipment has been applied subsequ ently for measuremen t at room tempera Lure of compression of a number of other mater ials tlmt fall in to the two general caLegories of high polymeric substances and minerals. Th e data on compression of minerals is primarily of geological intere L and will be reported elsewhere. The results of experiments on high polymers are of particular interest h ere and constitute the subj ect of this r eport.
II. Experimental Method and Treatment of Data
The apparatus and experimental procedure have been described in detail previously [1 , 2], and will not be discussed fully here. Briefl y, an experiment consists of forcing a leakproof piston into the bore of a heavy -walled cylinder , which contains the speci-men immersed in a suitable pressure-transmitting liquid (Varsol, a mixture of naphthenes boiling between 1500 and 200 0 C). Combination of the measurements of depth of penetration of the piston and the internal hydrostatic pressure- made at eaell 1,000 atm- with measurements obtained from a similar experimen t in which the specimen is replaced by a steel bar of comparable volume, permits a cal-culation of the compression of the specimen . Suit- able equations for th e calculation , as well as valu es of the cons tan ts of the vessel and the V arsolrcq uired, have been given previously [2, 1] .
I Figures in brackets indicate the li terature references at the end of this paper.
:MeasufemenL were mad e in t he pressure range 1,000 to 10,000 atm. T he upper limit of 10,000 atm was self-imposed a a re uJ t of a crack existing in the ram , while the lower limi t of 1,000 atm. is imposed in this type of experimen t by frictional forces between packing washers and the bore of the vessel.
The notation used here conforms to that followed for many years by workers at the Geophysical Lab-oratory of t he Carnegie Institu te of \'Vashington. The compression - Lll '/F o i defined as - (Vp - V') /V o, wh ere V p i the volume at pres m e P; V ' is the volume at the experimental refcrence pressure of 2,000 atm; and 110 is the initial volume at atmospheric pre sure. The subscript zero may be taken to refer to zero atmospheres, since in these and most other high-pressure measurements, the volume change oc(;urring between 0 and 1 atm is insignifi cant. The compres-sion occurring bctween 1 and 2,000 atm is clesign lJ..ted by - Ll V ' /Vo and is equal to - (V' - Vo) /Vo. This compression which is not measured in these experi-ments is referred to as the initial compression.
Estimation of the ini tial compression that occurs between 1 and 2,000 atm was made by successive extrapolations of tf'ntative calculations of compres-sion to 1 atm rath er than by t he least squares method previously described . While this extrapolation is not to be constru ed as more than mod erately ac-curate, it is believed sufficien tly accmate for the fol-lowing reason : The rcq uiTed initial compression enters the calculation in a correction term that is usually small. Errors in asse smen t of the initial compression of as mu ch as a few tenths of a percent result in negligible variation in the measmed values between 1,000 and 10,000 atm. However, if the compression is reckoned from 1 atm, the initial com-pression (- Ll F ' / Fo, 1 to 2,000 atm) must be added to the measured values, and the final res ults will be subj ect to at least as mu ch uncertainty as is involved in th e initial compression. To eliminate this uncer-
tainty, all da,ta and calculations are based on the experimental reference pressure of 2,000 atm, at which - f1 V / Vo is taken to be zero. Values at 1,000 atm therefore appear as negative compressions, which as a result of the previously mentioned fric-tional forces, are less reliable than data at higher pressures.
In the present experiments no serious attempt was made to establish the presence of slow plastic flow under hydrostatic pressure. Most observations made during measurements, however, indicate that if such a process occurs a much longer time than was used here must be employed for its detection. Pres-sure equilibrium in these measurements appeared to be obtained in 15 to 20 minutes following each pressure change, a period of time ordinarily required for establishment of thermal equilibrium . Ob-servations made during measurements were indica-tive of an instantaneous response to pressure changes in all specimens except Thiokol rubber. The agree-ment of data obtained in duplicate measurements made on some specimens also tends to indicate negligible permanen t set.
During the course of these experiments the dial gage, which was used to measure the depth of pene-tration of the piston, was remounted directly on the ram itself. Measurement.s with all rubber samples were made with this arrangement. All other data were obtained with the dial gage mounted on the top platen of the press.
III. Materials Studied There is a scarcity of data on behavior of all
polymeric materials in this pressure range, but the choice of materials to be studied was dictated by the Varsol used as the confining liquid. Only those available materials expected to be resistant to swell-ing by Varsol were studied. The following materials weTe investigated :
Gellulose.- A sample of purified cotton was com-pressed into cylindrical form for test and was dried at 100 C in vacuum 2 mm Hg) for 48 hours. This specimen is referred to as dry cellulose, and had a density of l.521 g/cm3 at 20 C, as measured by hydrostatic weighing in Varsol  .
Polytetrafluoroethylene (Teflon).- One sample of T eflon , denoted sample A, was an opaque, grey rod having a density of 2.236 g/cm3 at 20 C. The previous history of this sample is unknown. Sample B was obtained from the E. 1. Dupont de Nemours & Co., and was a rod of mottled greyish color having a density of 2.219 g/cm3 at 20 C. The mottled appearance was caused by dispersed dark material in the greyish bulk of the rod.
Polymonochlorotrifluoroethylene (Kel-F). *- A sheet of this material was available for test. The material was transparent with a sligh t opalescence and had a density of 3.168 g/cm3 at 20 C. A bundle of strips of suitable width, cut from the sheet, comprised the test specimen.
Polyethylene.-A molded rod, which served as test specimen, had a density of 0.917 g/cm3 at 20 C.
'This m aton aJ is of uncerta in origin and history .
Polyvinylidenechloride (Saran).- A sheet of this substance was available for study.
The material was very dark in color, and had a density of 1.099 g/cm3 at 20 C. A bundle of strips cut from the sheet formed the test specimen.
Polyester.- A molded rod of this material was made of Selectron 5003, and was a brittle rigid product having a slightly yellowish cast. The density was found to be 1.190 g/cm3 at 20 C .
All rubbers studied were raw stock containing no fillers or added vulcanizing agents, as follows:
Hycar OR25.- A molded cyclinder of density 0.972 g/cm3 at 20 C.
Hycar OR15.- A molded cylinder of density 0.964 g/cm3 at 20 C.
Neoprene.- A rough cylinder cut manually from an irregularly shaped piece of raw stock. This sample was probably partially crystalline, and had a density of 1.134 g/cm 3 at 20 C.
Thiokol ST.- A test specimen formed by stacking disks of rubber cut from an irregularly shaped piece of raw material. The density of the specimen was 1.298 g/cm3 at 20 C.
IV. Results and Discussion
1. Synthetic Plastics and Cellulose
The results of measurements made on cellulose, polyethylene, polymonochlorotrifluorethylene, poly-vinylidene chloride, and a polyester are given in table 1.